Recommendation of RILEM TC 212-ACD: acoustic emission and related NDE techniques for crack detection and damage evaluation in concrete*
- 2.2k Downloads
KeywordsAcoustic Emission Concrete Structure Shear Crack Acoustic Emission Signal Acoustic Emission Event
Concrete Structures are known to be no longer maintenance-free. Consequently, a variety of inspection techniques are under development and going to be established. It is well known that acoustic emission (AE) technique is promising to test concrete structures for damage estimation . For in-situ inspection, estimation of active cracks is of significant importance. Due to damage evolution in reinforced concrete structures, AE events are observed under in-service conditions. Generally speaking, nucleation of shear cracks follows tensile cracks on an existing failure surface. Accordingly, for an early warning of crack nucleation, the classification of active cracks is in great demand. In this recommendation, a classification criterion for micro-cracks in concrete is proposed on the basis of the measurement of AE parameters
2 Definition of technical terms
Peak amplitude: Largest amplitude value in a waveform.
Rise time: A duration time from the first arrival to the peak amplitude.
Duration time: Duration observed from the first arrival to the time when the amplitude decays up to the level lower than the threshold.
Counts: Normally, AE counts imply number of times the signal amplitude exceeds the threshold. They also are rigorously named ring-down counts.
External parameters: The measurement system shall be able to obtain time information along with AE parameters. In addition, such external parameters as load, strain and so forth are preferably recorded in the system.
3 Measurement system
3.1 AE sensor
AE sensors shall be calibrated properly in advance of the measurement. AE sensor is sensitive enough to detect AE signals generated in a concrete structure, taking acoustic coupling into consideration. AE sensor is also robust enough against temperature change, moisture condition and mechanical vibrations in the environments.
For the parameter analysis, a broad-band sensor is recommended. But, resonance-type sensors are also available, in the case that their resonance frequencies are higher than 60 kHz in concrete. So far, resonant frequencies of resonance-type sensors have been applied to concrete in the range of 50–250 kHz.
3.2 System for signal analysis
The system of AE devices shall be specified, depending on the target. AE sensors are attached at proper locations to cover the target area. The internal noise of the amplifier shall be inherently low and less than 20 μV (26 dB for 0 dB = 1 μV) as the peak voltage converted by input voltage. The amplifier shall be robust enough against the environmental conditions and be protected properly. The frequency range shall be determined prior to the measurement, taking into account the performance of AE sensor and the amplifier. The range from several kHz to several 100 kHz is recommended in concrete. The period of the measurement shall be prescribed, depending on propagation property of AE signals in the target structure.
4 Environmental noises
In advance to AE measurement, the noise level shall be estimated. Then, counteract against external noises, wind, rain, sunshine and so forth shall be conducted to decrease the noise level as low as possible. In the case that the noises have similar frequency contents, amplitudes to AE signals or sources of the noises are unknown, characteristics of the noises shall be estimated prior to the measurement. Based on this result, separation of AE signals from the noises shall be achieved. In this respect, the use of filters is applicable after determining the proper frequency range.
Sensitivity of AE channels shall be conducted routinely by employing the standard source. Variation within the channels shall be less than 3%.
5 Test procedure
AE signals due to cracking shall be detected properly for the duration of the measurement. The test shall be conducted under loads which must not fundamentally make any critical damage on functions of the structure to detect and locate active cracks. In advance to the test, attenuation properties of the target structure shall be estimated, by employing the standard source or the equivalent.
For plotting data, the ordinate is shown by physical unit of kHz and the abscissa scale is msec/volt, where the amplitude shall be calibrated as the sensor output, compensating the effect of amplifiers. In the figure, the ratio of the abscissa scale to the ordinate scale is set to 10. But, it just means a suggestive value. A proper ratio shall be determined, depending on materials and structures. It is recommended to set the ratio in advance to the classification of active cracks. In a reference, it is recommended to apply the ratio of 50, based on the moment tensor analysis . In another reference, just a trend of these two indices (1) and (2) is applied to identify the corrosion process in reinforced concrete , and to characterize the transition from tensile to shear cracking in steel-fiber reinforced concrete .
Results of system inspection before and after the setup
- 1.Grosse CU, Ohtsu M (eds) (2008) Acoustic emission testing. Springer, 2008Google Scholar
- 2.European Norms: EN1330-9 Nondestructive testing—terminology-Part 9: terms used in AE testingGoogle Scholar
- 3.EN 13554 Nondestructive testing-Acoustic emission-General principlesGoogle Scholar
- 4.American Society for Testing and Materials (ASTM) E1316 Standard Definitions of Terms relating to AEGoogle Scholar
- 5.ASTM E650 Standard Guide for Mounting Piezoelectric AE SensorsGoogle Scholar
- 6.ASTM E750 Standard Practice for Characterizing AE InstrumentationGoogle Scholar
- 7.American Society for Nondestructive Testing (ASNT) DGZfP-SE1 nondestructive testing: acoustic emission termsGoogle Scholar
- 8.ASNT DGZfP-SE3 Guide line for AE Characterization during AE TestGoogle Scholar
- 9.French Association for Standards (AFNOR) NF A09-350 nondestructive testing-vocabulary used in acoustic emissionGoogle Scholar
- 10.European Working Group on Acoustic Emission (EWGAE) Codes for AE examination: code I-location of discrete acoustic eventsGoogle Scholar
- 11.EWGAE Codes for AE Examination: code IV-definition of terms in AEGoogle Scholar
- 12.Japanese Society for Nondestructive Inspection (JSNDI) NDIS 2421 Recommendation practice for in situ monitoring AE of concrete structures by AEGoogle Scholar
- 13.Ohno K, Ohtsu M (2008) Comparison of crack classification in concrete by parameter analysis and SiGMA in acoustic emission, Proc. structural faults and repair 2008, 12th international conference and exhibition. Edinburgh, UK (CD-ROM)Google Scholar
- 14.Ohtsu M, Tomoda Y (2008) Phenomenological model of corrosion process in reinforced concrete identified by acoustic emission. ACI Mater J 105(2):194–199Google Scholar